BUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION


 Wilfred Cooper
 1 years ago
 Views:
Transcription
1 2 th International Conference on Composite Materials Copenhagen, th July 215 BUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION José Humberto S. Almeida Jr. 1, Marcelo L. Ribeiro 2, Volnei Tita 2, Hugo Faria 3, António T. Marques 4, Sandro C. Amico 1 1 PPGE3M, Federal University of Rio Grande do Sul, Av. Bento Gonçalves, Porto Alegre, RS, Brazil 2 Department of Aeronautical Engineering, Engineering School of São Carlos, University of São Paulo, Av. João Dagnone 11, São Carlos, SP, Brazil 3 Composite Materials Unit, INEGI  Institute of Mechanical Engineering and Industrial Management, Rua Dr. Roberto Frias 4, , Porto, Portugal 4 FEUP  Faculty of Engineering of the University of Porto, Rua Dr. Roberto Frias s/n, , Porto, Portugal Keywords: buckling, composite tubes, filament winding, postbuckling, progressive failure ABSTRACT Transverse compression (ring deflection) tests were simulated in composite tubes through nonlinear finite element models based on a modified Riks algorithm, which uses the arclength method. Progressive failure was evaluated in detail through a proposed damage model, able to identify the failure mode. In all composite tubes tested, localized stress concentration points developed in the transverse plane caused by contact load plates/composite, producing nonlinearity in the load vs. displacement curves (P ). The failure mode of these tubes involves a complex combination of mechanisms, namely transverse tensile, transverse compression and inplane shear stresses, where the region of the specimen in contact with the load plates present the most damaged area. Thus, matrix tensile and matrix compression induced by shear near the loading zones dominate damage and failure of the specimens. Buckling and postbuckling of tubes are highly influenced by the fiber orientation, whereas the tube with reinforcement orientation parallel to the loading platestospecimens contact line withstanding the highest buckling load level. On the other hand, specimens wound at [±45] 5 and [±75] 5 present a divergence point, since they support a portion of the load after buckling is reached, characterizing a postbuckling behavior. 1 INTRODUCTION Cylindrical shells have numerous applications in aerospace, aeronautic and marine structures, such as in launch vehicle fuel tanks, fuselages and offshore structures. They have the ability to carry high levels of axial and transverse compression, since most of the structure is loaded in a membrane state and its efficiency is derived from the lack of throughthethickness stress gradients [1]. These structures are traditionally metallicbased, therefore due to the evergrowing need to decrease the payload in such aeronautic and marine structures, the use of polymeric composites is being motivated, mainly due to their high corrosion resistance and high stiffness and strengthtoweight ratios. Filament winding (FW) process stands out in composite materials processing because of its high precision in fiber positioning, high fiber content, high automation capability and low void content. Due to these characteristics, FW is the most common process for manufacturing revolution and axisymmetric parts, such as composite overwrapped pressure vessels and tubes. When these structures
2 José Humberto S. Almeida Jr., Marcelo L. Ribeiro, Volnei Tita, Hugo Faria, António T. Marques, Sandro C. Amico act under uniaxial or biaxial load, as the load increases steadily, the shell starts to deform stably. When the load achieves a critical point, the equilibrium stops and instability may be set. Thus, buckling occurs when the structure suddenly deflects unstably and loses its capacity to keep resisting the compressive loading. Fig. 1 shows a typical load vs. displacement response for an unstable problem. Composite tubes with a sufficiently thinwall shell fail due to either global or local buckling when under an instable loading, and they have two possible distinct characteristics: the first one is that the development of significant radial and/or axial displacements is followed by the development of global buckling phenomena and a consequently collapse; and the second one is that the prediction of the load level at which collapse occurs is difficult when compared to wellbehaved structures, such as beams and plates [1,2]. Figure 1: Typical response of a structure under unstable loading [3]. It is common to find researches dealing with isotropic and even composite tubes under axial compression [4,5,6], which is the most classical case of a structure under an instable loading that causes buckling. However, there are no reports about the buckling behavior of composite cylindrical shells under transverse compression, which can be relevant for tubes acting under either transverse compression or hydrostatic external pressure. In both cases, the structure can fail by buckling or material failure, where they are strongly dependent of the stacking sequence, wall thickness, boundary conditions or geometrical imperfections [7]. In some cases, the structure can support a portion of the applied loading after buckling is reached, formerly known as postbuckling, typical of isotropic metallic structures. However, a composite structure may also present a postbuckling behavior even with its brittle fracture behavior. For instance, White et al. [1] performed the postbuckling analysis of variablestiffness cylindrical shells under axial compression through linear and nonlinear analysis, where both presented results within the error range achieved in experimental results, but the nonlinear analysis predicted better the final postbuckled shape. Tafreshi [2] developed a numerical model to predict the buckling and postbuckling behavior of composite cylinders under external pressure and axial compression, where the delamination was the main cause of the buckling. Harte and Fleck [8] investigated the failure behavior of braided composite cylinders under axial compression and torsion, where different failure modes were successfully predicted in the developed models. In this context, this work deals with the development of reliable models to represent the buckling and postbuckling behavior of composite tubes under transverse compression (also referred to as ring deflection). Two strategies have been implemented: i) geometrically nonlinear analyses and ii) advanced damage modelling. 2 BASICS OF BUCKLING 2.1 Linear buckling analysis Firstly, a linear Eigenvalue buckling analysis was carried out aiming at determining the buckling
3 2 th International Conference on Composite Materials Copenhagen, th July 215 critical load and the deformed shape for the composite tubes under transverse compression. The essence of an eigenvalue buckling problem is to find the loads where the stiffness matrix becomes singular, and thus the problem has nontrivial solutions [9], being represented by Eq. 1: K mn υ m = (1) where K mn is the tangent stiffness matrix when the load is applied and υ m are nontrivial displacement solutions. In the linear buckling analysis, a perturbation is applied to the undeformed shape of the specimen. Specified sets of loadings are monitored for which deflections could induce instability when under a geometric nonlinearity (also known as PDelta, P, effect), which involves the equilibrium and compatibility relationships of a structural system loaded about its deflected configuration [3]. Linear buckling procedure generates a range of buckling factors and corresponding mode shapes. When loading is multiplied by these buckling factors, the resulting scaled loading conditions represent those that induce buckling. Similarly, the mode shapes are normalized displacement sets which indicate the configuration of the buckled structure [1,11]. 2.2 Nonlinear buckling and postbuckling analysis In order to evaluate both buckling and postbuckling of the structure, a nonlinear buckling model is suitable to provide more accurate results than the elastic formulation. In this analysis, an applied loading incrementally increases until a large change in displacement occurs for a certain increment. This condition typically points that the structure has become unstable. Nonlinear buckling analysis is a static method that accounts for material and geometric nonlinearity, load perturbations and/or geometric imperfections. Geometrically nonlinear static problems occasionally involve buckling or collapse behavior, where the loaddisplacement response displays a negative stiffness and the structure should release strain energy to remain in equilibrium [2]. Buckling analysis commonly provides a bifurcation after the structure loses its equilibrium, but even in snapthrough problems (equilibrium path in loaddisplacement space is smoothed and does not branch) the Riks algorithm may be employed. In case of a snapthrough behavior, the structure can carry increasing load after a complete snap [12]. 3 MATERIAL MODEL This material model was originally developed by Ribeiro et al. [7] at a mesoscale approach, where it was adapted to the material and geometry herein used. The model regards to the composite lamina under plane stress state and the damage is considered uniform throughout the laminate thickness [13]. 3.1 Fiber modelling A unidirectional carbon/epoxy composite laminate under tensile loading in the fiber direction (σ 11 ) is linear elastic with brittle fracture. Thus, for tensile load in fiber direction, the maximum stress criterion is used to identify the fiber failure: σ 11 X t 1 (1) After failure is reached, the damage variable in fiber direction (d 1 ) is set to.99. There is no evolution of d 1 aiming at represent the catastrophic failure of the carbon fiber. To avoid possible localization issues, the degradation of properties is calculated in the step i, however it is applied into the step i + 1, thus improving the convergence process. The fiber behavior under compressive longitudinal load is set to be linear elastic until a specified value, after that, a nonlinear elastic behavior is observed. The linear elastic to nonlinear elastic limit (X C ) is then used in Eq. 2 to represent the compressive failure, as follows: σ 11 X C 1 (2) After σ 11 X C any increase in the compression loads in fiber direction results in a nonlinear
4 José Humberto S. Almeida Jr., Marcelo L. Ribeiro, Volnei Tita, Hugo Faria, António T. Marques, Sandro C. Amico elastic stress strain behavior. This nonlinear elastic behavior is simulated using a secant modulus as can be seen in Eq. 3: E 11 = X C ε 11 (1 h(ε 11)) + h(ε 11 )E 11 (3) Where h(ε 11 ) is obtained from the fit of stressstrain plots for specimens under compressive loading, ε 11 is the strain in longitudinal direction and E 11 is the initial elastic modulus from specimens under compression loading. 3.2 Matrix modelling In a unidirectional quasiflat filament wound laminate, the damage process in the matrix is essentially dominated by the transverse loading (σ 22 ) and shear loading (τ 12 ). A nonlinear behavior in the matrix is reported due to inelastic strains and damage in matrix [14]. To model the damage process in matrix, two internal damage variables, d 2 (related to σ 22 ) and d 6 (related to τ 12 ), were used. Based on Continuous Damage Mechanics, the hypothesis of effective stress links the damage variables to the stresses [9], and Eq. 4 gives the relationship σ 11 { σ 22 } = τ 12 [ 1 1 d1 1 1 d2 1 1 d6 ] σ 11 { σ 22 } (4) τ 12 where σ ij τ ij are the second order effective stress tensors. According to Herakovich [9], the damage strain energy density can be described in function of effective stresses considering only for matrix phase stresses, as shows Eq. (5) E D = 1 [ σ σ 22 2 E 22 (1 d 2) E 22 + τ 12 2 ] (5) G 12 (1 d 6 ) where σ = σ 22 if σ 2 22 >, otherwise σ = if σ 2 22 <. Similarly, σ = σ 22 if σ 2 22 <, otherwise σ 2 22 = if σ 2 22 >. Another aspect of the present model must be highlighted, which consists in an adjustment of the Poisson s coefficient for consider the damage effect. Using CDM formulation performed by Matzenmiller et al. [15], Eq. 8 gives the compliance tensor: D = 1 K [ (1 d 1 )E 11 (1 d 1 )(1 d 2 )ν 21 E 22 (1 d 1 )(1 d 2 )ν 12 E 11 (1 d 2 )E 22 K(1 d 6 )G 12 ] (8) where, K = (1 (1 d 1 )(1 d 2 )ν 12 ν 21. Aiming at avoiding the material selfhealing, the damage parameters (d 1, d 2 e d 6 ) are assumed as the maximum.99 along the simulation [7]. 4 FINITE ELEMENT MODELLING The herein presented models were built up in Abaqus 6.14 software platform. The original dimensions of the tubes are: length (l) = 381 mm, radius (r) = 68 mm and lamina thickness (t l ).6 mm (t l varies according to winding angle). The structure was modeled with S4R shell elements with three integration points in each layer. The cylindrical shell has been submitted to a transverse compressive load by contact from the compression plates (rigid bodies). Fig. 3 depicts the assembly of the virtual test. The tubes were modelled by using four node reduced integration shell element (S4R) with hourglass control. Table 1 presents the comprehensive material properties of the carbon/epoxy laminates. A compressive load was applied into the top compressive plate (rigid body) and the other plate is clamped. The buckling loading was transmitted to the specimen by contact from the rigid bodies. A modified Riks algorithm based on the arclength method was used to predict is buckling and/or postbuckling occurs. Figure 2 presents the assembly of the virtual test.
5 2 th International Conference on Composite Materials Copenhagen, th July 215 Elastic constants Strengths E 1 (GPa) E 2 = E 3 (GPa) G 12 = G 13 (GPa) 5.44 G 23 (GPa) 2.1 X t (MPa) X c (MPa) 74. Y t (MPa) 42.5 Y c (MPa) 14.3 S 12 (MPa) 68.9 Table 1: Material properties used as input in the numerical models. 4.1 Parametric study Figure 2: Assembly of the transverse compression test. A parametric study was carried out aiming at evaluate the mechanical response of the tube with different winding sequence and radius/thickness (r/t) ratios. Table 1 shows all configurations used in the simulations. Specimen code Stacking sequence r/t ratio [±45] 5 [±45] 5 [±75] 5 [±75] [±9] 5 [9] 5 r/t_22.7 [9] r/t_28.3 [9] r/t_37.7 [9] Table 2: Description of all specimen configurations used for the parametric study. 5 RESULTS AND DISCUSSION Figure 3 presents the linearelastic simulations to identify the global mechanical response of the tubes with different winding angles under transverse compression. The tube wound with hoop layers ([9] 5 ) supports higher compressive load than the other layups simulated. This performance was foreseen since the composite tube is loaded in fiber (hoop) direction. Even with geometric nonlinearity activated in the model, it is obvious that no buckling happens, where all specimens supported the
6 Load proportionality factor Load (N) José Humberto S. Almeida Jr., Marcelo L. Ribeiro, Volnei Tita, Hugo Faria, António T. Marques, Sandro C. Amico applied load until the maximum displacement set. Displacement (mm) [±45]5 [±75]5 [±9]56 Figure 3: Load displacement curves for the three winding angle evaluated through a nonlinear elastic analysis with geometric nonlinearity activated. Figure 4 shows the load proportionality factor (LPF) vs. total arc length of the simulations through a nodal analysis, aiming at finding the bifurcation point and critical buckling load for the tubes analyzed. In these plots, the values are not relevant, however the curve shape reveals the geometrical instability throughout the analysis. As can be noted, the fiber orientation influences directly on the compressive behavior of composite tubes, since the specimen [9] 5 present a clear buckling load without evidence of postbuckling, considering that when the structure buckles the analysis converges to a unique solution, a failure by buckling. On the other hand, the specimens [±45] 5 and [±75] 5 do not present a clear buckling load, but it is possible to find a bifurcation point due to the nonlinear shape of the curves. Arc length [±45]5 [±75]5 [±9]52.5 Figure 4: Load proportionality factor vs. arc length obtained from the nodal analysis for identify the buckling load and bifurcation point. Figure 5 may complement previous results obtained from Figure 4, showing the load vs. displacement plots for the cylinders. Specimen [±45] 5 presents a slightly drop at around 2 kn with a displacement of 4 mm, which can be find as a bifurcation point, to be confirmed by analyzing the material failure. The cylinder wound at [±75] 5 is the sequence that presents less influence of buckling,
7 Load (N) 2 th International Conference on Composite Materials Copenhagen, th July 215 since the cylinder start to behave slightly instable after a displacement of 3 mm. The specimen [9] 5 loses its structural integrity at 44.7 kn, being that the buckling load. Displacement (mm) [±45]5 [±75]5 [±9] Figure 5: Load displacement profile curves for the tubes with different winding angle through a nodal analysis. Analyzing the shape of the cylinders in an increment that the structure starts to lose structural stability (Figure 6), it is clear that the tubes are too dependent of the fiber orientation, since the hoop wound tube presents a typical mode I of buckling under a compressive load. However, it cannot be stated that any of these structures may failed buckling. For that, a failure evaluation seems crucial to understand the complete behavior of these structures under an unstable load. Figure 6: Deformed shape of the tubes at the increment in which the structure starts to be unstable. 5.1 Failure and damage analysis Figure 7 presents the progressive failure analysis for the tubes exhibited through the load vs. displacement curves. As can be noted, the tube [9] 5 presented a sudden failure at 25 kn with a displacement 2.7 mm. Although Riks analysis pointed a buckling load of 44.7 kn, the failure analysis evidences that the tube fails by material failure before achieve the buckling load. The specimen [±45] 5 has a bifurcation point at a load of 18.1 kn at the displacement of 38.2 mm, which is similar to buckling load found at the nodal analysis. This curve shape suggests a postbuckling behavior, since the specimen does not fail at the buckling load, since the structure keep carrying a portion of the compressive load. The tube [±75] 5 points a bifurcation at a load of 24.5 kn and displacement of 35.7 mm, but with a large amount of failed plies, characterizing that the structure postbuckles but with various plies damaged. It is interesting to observed in these load vs. displacement profiles that the curves fluctuate along the analysis with several tiny discontinuities, which may correspond to progressive failure of the plies. A typical issue in these test is the contact between the rigid plates and the composite specimen, since
8 Load (N) Load (N) José Humberto S. Almeida Jr., Marcelo L. Ribeiro, Volnei Tita, Hugo Faria, António T. Marques, Sandro C. Amico this contact may induce a transverse shear between them, being cause a premature failure of the specimen. Displacement (mm) First matrixdominated ply failed Ultimate and fiberdominated failure 51 Matrixdominated elements failed Bifurcation point [±45]5 [±75]5 [±9]5 Material failure 3 Figure 7: Mechanical response of the tubes simulated by using the damage model herein proposed. It is observed a high dependence of the winding angle on the failure of the specimens under the compressive load. As the winding angle increases, the failure load increases. The analysis indicate that when the fiber orientation is aligned perpendicular to the loading axis, the cylinder become more stable under transversal compressive loading. Thus, with fibers wound in the hoop direction, the tube is more able to sustain higher hoop stress levels prior to failure. 5.2 Parametric study Figure 7 shows typical curves for the tube [9] 5 with different radiustothickness (r/t) ratios. As the r/t ratio increase, the buckling load decreases, once as thinner as the wall thickness the structure becomes more susceptible to buckling. In addition, as higher as the r/t ratio, the specimen displace more at a lower maximum peak load. The specimen r/t_37.7 has the most instability throughout the analysis, which can be attributed to the high influence of transverse shear stresses. Despite at different loads, a similar profile is observed for each tube until 2 mm, presenting a linear response. The deviation from linearity to nonlinearity is clear for all specimens, even though at different load stages indicating active damage mechanisms in all tubes r/t_22.7 r/t_ Displacement (mm) 3 Figure 8: Mechanical response for the cylinders with several radiustothickness ratios.
9 2 th International Conference on Composite Materials Copenhagen, th July 215 The deformed shape of these tubes at the failure load is shown in Figure 9, where the thinnest tube present a bifurcation point at a load of 7.8 kn and a displacement of 25 mm, being this the reason for a high displacement by supporting a small portion of the load (compared to the other tubes). This cylinder has a matrixdominated failure mode, mainly by transverse shear and transverse tensile stresses. It is valid to mention the stress concentrations created at the contact plate/specimen, however this cylinder does not present fiberdominated failure. Figure 9: Final deformed shape of each tube and their spatial displacement in the circumferential direction. 6 CONCLUSIONS The scope of this paper was to evaluate the buckling and/or postbuckling response of filament wound composite tubes under a transversal compressive load. For that, a nonlinear analysis based on a modified arclength method was used to predict the buckling load and the bifurcation point. In addition, a damage model was proposed, in order to understand the progressive failure and damage upon buckling onset of the tubes with several winding angle and radiustothickness ratio. The specimen wound with hoop layers supported the highest compressive load, pointing a buckling load of about 4 kn, whereas the tubes [±45] 5 and [±75] 5 have a bifurcation point in lower loads, presenting a postbuckling behavior, since the structure still support portion of the load of buckling is reached. However, the specimen [9] 5 failed in the material before a buckling load, with a combination of transverse tensile, inplane shear and radial compression, beyond a few fiberdominated failures at the contact between the rigid plates and composite specimen, being this point the final failure location. The failure analysis corroborated that the [±45] 5 and [±75] 5 present postbuckling after a displacement at around 4 mm, and the tube [9] 5 did not show postbuckling. The next step of this research is to carry out the experiments to validate the buckling and postbuckling models herein developed, as well as the damage model and progressive failure of the plies during this test. ACKNOWLEDGEMENTS The authors are grateful to CAPES, CNPq, AEB (Brazilian Space Agency) and CCDRN (Portugal) for the financial support to this study, through corresponding cofunded programs. REFERENCES [1] S.C. White, P.P. Weaver, K.C. Wu, Postbuckling analyses of variablestiffness composite cylinders in axial compression, Composite Structures, 123, 215, pp (doi: 1.116/j.compstruct ). [2] A. Tafreshi, Delamination buckling and postbuckling in composite cylindrical shells under combined axial compression and external pressure, Composite Structures, 72(4), 26, pp (doi: 1.116/j.compstruct ).
10 José Humberto S. Almeida Jr., Marcelo L. Ribeiro, Volnei Tita, Hugo Faria, António T. Marques, Sandro C. Amico [3] Dassault Systèmes Simulia Corporation, Abaqus 6.13, Analysis User's Guide, Providence, RI, USA, 214. [4] A. Tafreshi, Efficient modelling of delamination buckling in composite cylindrical shells under axial compression, Composite Structures, 64(34), 24, pp (doi: 1.116/j.compstruct ). [5] C. Bisagni and P. Cordisco, An experimental investigation into the buckling and postbuckling of CFRP shells under combined axial and torsion loading, Composite Structures, 6(4), 23, pp (doi: 1.116/S (3)242). [6] T. von Kármán and HS. Tsien, The Buckling of Thin Cylindrical Shells under Axial Compression, Journal of Spacecraft and Rockets, 4(6), 23, pp (doi: /2.756). [7] M. Życzkowsky, Postbuckling analysis of nonprismatic columns under general behaviour of loading, International Journal of NonLinear Mechanics, 4(4), 25, pp (doi: 1.116/j.ijnonlinmec ). [8] AM. Harte and N.A. Fleck, Deformation and failure mechanisms of braided composite tubes in compression and torsion, Acta Materialia, 48(6), 2, pp (doi: 1.116/S (99)4279). [9] S. Novoselac, T. Ergić, P. Baličević, Linear and nonlinear buckling and post buckling analysis of a bar with the influence of imperfections, Tehnički Vjesnik, 19(3), 212, pp [1] M.W. Hilburger and J.H. Starnes Jr, Effects of imperfections on the buckling response of compressionloaded composite shells, International Journal of NonLinear Mechanics, 37(45), 22, pp (doi: 1.116/S27462(1)889). [11] V.V. Bolotin, Delamination in composite structures: its origin, buckling, growth and stability. Composites Part B, 27(2), 1996, pp (doi: 1.116/ (95)356). [12] E. Riks, An incremental approach to the solution of snapping and buckling problems, International Journal of Solids and Structures, 15(7), 1979, pp (doi: 1.116/27683(79)9817). [13] C. Herakovich, Mechanics of fibrous composites, Vol. 1, Wiley Publisher, [14] A. Puck, H. Schürmann, Failure analysis of FRP laminates by means of physically based phenomenological models, Composites Science and Technology, 58(7), 1998, pp (doi: 1.116/S (1)281). [15] A. Matzenmiller, J. Lubliner, R.L. Taylor, A constitutive model for anisotropic damage in fibercomposites, Mechanics of Materials, 2(2), 1995, pp (doi: 1.116/ (94)53).
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationREPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 REPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
More informationCrashworthy Design of Composite Structures Using CAE Process Chain
0 th European LSDYNA Conference 205, Würzburg, Germany Crashworthy Design of Composite Structures Using CAE Process Chain Madhukar Chatiri, Thorsten Schuetz 2, Anton Matzenmiller 3 CADFEM GmbH, Grafing
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationSIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS
VOL. 5, NO. 4, APRIL 010 ISSN 18196608 006010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationAim of the study Experimental determination of mechanical parameters Local buckling (wrinkling) Failure maps Optimization of sandwich panels
METNET Workshop October 1112, 2009, Poznań, Poland Experimental and numerical analysis of sandwich metal panels Zbigniew Pozorski, Monika ChudaKowalska, Robert Studziński, Andrzej Garstecki Poznan University
More informationLINEAR AND NONLINEAR BUCKLING ANALYSIS OF STIFFENED CYLINDRICAL SUBMARINE HULL
LINEAR AND NONLINEAR BUCKLING ANALYSIS OF STIFFENED CYLINDRICAL SUBMARINE HULL SREELATHA P.R * M.Tech. Student, Computer Aided Structural Engineering, M A College of Engineering, Kothamangalam 686 666,
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationITE IMPACT ON. Summary. concurrent. phenomena delamination. subroutine. simulations discussed. Keywords: Volnei Tita.
NUMERICAL AND EXPERIMENTAL ANALYSES OF LOW VELOCITY IMPACT ON THIN COMPOS ITE Marcelo L. Ribeiro Department of Aeronautical Engineeringg Engineering Scholl of São Carlos University of São S Paulo malribei@usp.
More informationPLY WAVINESS ON INPLANE STIFFNESS OF COMPOSITE LAMINATES
PLY WAVINESS ON INPLANE STIFFNESS OF COMPOSITE LAMINATES Cimini Jr., Carlos A., and Tsai, Stephen W. 2 Department of Mechanical Engineering, Federal University of Minas Gerais Av. Antônio Carlos, 6627
More informationAnalysis of asymmetric radial deformation in pipe with local wall thinning under internal pressure using strain energy method
Analysis of asymmetric radial deformation in pipe with local wall thinning under internal pressure using strain energy method V.M.F. Nascimento Departameto de ngenharia Mecânica TM, UFF, Rio de Janeiro
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationA Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber
A Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber Kibong Han Mechatronics Department, Jungwon University, 85 Munmuro, Goesangun, South Korea.
More informationINFLUENCE OF WEB THICKNESS REDUCTION IN THE SHEAR RESISTANCE OF NONPRISMATIC TAPERED PLATE GIRDERS
INFLUENCE OF WEB THICKNESS REDUCTION IN THE SHEAR RESISTANCE OF NONPRISMATIC TAPERED PLATE GIRDERS Paulo J. S. Cruz 1, Lúcio Lourenço 1, Hélder Quintela 2 and Manuel F. Santos 2 1 Department of Civil
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationNONLINEAR LOCAL BENDING RESPONSE AND BULGING FACTORS FOR LONGITUDINAL AND CIRCUMFERENTIAL CRACKS IN PRESSURIZED CYLINDRICAL SHELLS
NONINEAR OA BENDING RESPONSE AND BUGING FATORS FOR ONGITUDINA AND IRUMFERENTIA RAKS IN PRESSURIZED YINDRIA SHES Richard D. Young, * heryl A. Rose, * and James H. Starnes, Jr. NASA angley Research enter
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationCOROTATIONAL NONLINEAR DYNAMIC ANALYSIS OF LAMINATED COMPOSITE SHELL STRUCTURES
Copyright c 009 by ABCM January 0408, 010, Foz do Iguaçu, PR, Brazil COROTATIONAL NONLINEAR DYNAMIC ANALYSIS OF LAMINATED COMPOSITE SHELL STRUCTURES Felipe Schaedler de Almeida, schaedleralmeida@gmail.com
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationAE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF HOOP STRESSES FOR A THINWALL PRESSURE VESSEL
Objective AE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF OOP STRESSES FOR A TINWA PRESSURE VESSE This experiment will allow you to investigate hoop and axial stress/strain relations
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationThe Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints
, June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More information6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS
6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS Blondet et al. [25] carried out a cyclic test on an adobe wall to reproduce its seismic response and damage pattern under inplane loads. The displacement
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationSemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials
International Journal of Composite Materials 2017, 7(3): 103114 DOI: 10.5923/j.cmaterials.20170703.03 SemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials S. W. Chung 1,*, G. S. Ju
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationReference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity",
Reference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity", Oxford University Press, Oxford. J. Lubliner, "Plasticity
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationFASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES G. Catalanotti 1*, P.P. Camanho 1, P. Ghys 2, A.T. Marques 1 1 DEMec, Faculdade de Engenharia, Universidade
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationStrength of Material. Shear Strain. Dr. Attaullah Shah
Strength of Material Shear Strain Dr. Attaullah Shah Shear Strain TRIAXIAL DEFORMATION Poisson's Ratio Relationship Between E, G, and ν BIAXIAL DEFORMATION Bulk Modulus of Elasticity or Modulus of Volume
More informationPressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials
Pressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials Pressure Vessels: In the previous lectures we have discussed elements subjected
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationNonlinear Buckling Prediction in ANSYS. August 2009
Nonlinear Buckling Prediction in ANSYS August 2009 Buckling Overview Prediction of buckling of engineering structures is a challenging problem for several reasons: A real structure contains imperfections
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationSpherical Pressure Vessels
Spherical Pressure Vessels Pressure vessels are closed structures containing liquids or gases under essure. Examples include tanks, pipes, essurized cabins, etc. Shell structures : When essure vessels
More informationEsben Byskov. Elementary Continuum. Mechanics for Everyone. With Applications to Structural Mechanics. Springer
Esben Byskov Elementary Continuum Mechanics for Everyone With Applications to Structural Mechanics Springer Contents Preface v Contents ix Introduction What Is Continuum Mechanics? "I Need Continuum Mechanics
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More informationS. Srinivasan, Technip Offshore, Inc., Houston, TX
9 th ASCE Specialty Conerence on Probabilistic Mechanics and Structural Reliability PROBABILISTIC FAILURE PREDICTION OF FILAMENTWOUND GLASSFIBER Abstract REINFORCED COMPOSITE TUBES UNDER BIAXIAL LOADING
More informationSize Effects In the Crushing of Honeycomb Structures
45th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics & Materials Conference 1922 April 2004, Palm Springs, California AIAA 20041640 Size Effects In the Crushing of Honeycomb Structures Erik C.
More informationFinite ElementBased Failure Models for Carbon/Epoxy Tape Composites
Finite ElementBased Failure Models for Carbon/Epoxy Tape Composites A Master Thesis Presented to The Academic Faculty by Guillaume Seon In Partial Fulfillment of the Requirements for the Degree Master
More informationNUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION
NUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION Fabrice PIERRON*, François CERISIER*, and Michel GRÉDIAC** * SMS/ Département Mécanique et Matériaux, École Nationale Supérieure
More informationThe Local Web Buckling Strength of Coped Steel IBeam. ABSTRACT : When a beam flange is coped to allow clearance at the
The Local Web Buckling Strength of Coped Steel IBeam Michael C. H. Yam 1 Member, ASCE Angus C. C. Lam Associate Member, ASCE, V. P. IU and J. J. R. Cheng 3 Members, ASCE ABSTRACT : When a beam flange
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More informationModeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites
Modeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites H.E.Pettermann 1, C.Schuecker 1, D.H.Pahr 2, F.G.Rammerstorfer 2 1 Austrian Aeronautics
More informationGLOBAL AND LOCAL LINEAR BUCKLING BEHAVIOR OF A CHIRAL CELLULAR STRUCTURE
GLOBAL AND LOCAL LINEAR BUCKLING BEHAVIOR OF A CHIRAL CELLULAR STRUCTURE Alessandro Spadoni, Massimo Ruzzene School of Aerospace Engineering Georgia Institute of Technology Atlanta, GA 30332 Fabrizio Scarpa
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationFailure from static loading
Failure from static loading Topics Quiz /1/07 Failures from static loading Reading Chapter 5 Homework HW 3 due /1 HW 4 due /8 What is Failure? Failure any change in a machine part which makes it unable
More informationPrediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads
Prediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads J. Raju 1*, D.S. Sreedhar 2, & C.M. Manjunatha 1 1
More informationINFLUENCE OF FLANGE STIFFNESS ON DUCTILITY BEHAVIOUR OF PLATE GIRDER
International Journal of Civil Structural 6 Environmental And Infrastructure Engineering Research Vol.1, Issue.1 (2011) 115 TJPRC Pvt. Ltd.,. INFLUENCE OF FLANGE STIFFNESS ON DUCTILITY BEHAVIOUR OF PLATE
More informationMechanical Design in Optical Engineering
OPTI Buckling Buckling and Stability: As we learned in the previous lectures, structures may fail in a variety of ways, depending on the materials, load and support conditions. We had two primary concerns:
More informationMECHANICAL CHARACTERISTICS OF CARBON FIBER YACHT MASTS
MECHANICAL CHARACTERISTICS OF CARBON FIBER YACHT MASTS This paper provides a preliminary stress analysis of a carbon reinforced layered cylinder such as would be found in a yacht mast. The cylinder is
More informationA Multinodal Ring Finite Element for Analysis of Pipe Deflection
A Multinodal Ring Finite Element for Analysis of Pipe Deflection 109 A Multinodal Ring Finite Element for Analysis of Pipe Deflection E.M.M. Fonseca 1, F.J.M.Q. de Melo and M.L.R. Madureira 3 1 Department
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationLectures on. Constitutive Modelling of Arteries. Ray Ogden
Lectures on Constitutive Modelling of Arteries Ray Ogden University of Aberdeen Xi an Jiaotong University April 2011 Overview of the Ingredients of Continuum Mechanics needed in Soft Tissue Biomechanics
More informationUNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation.
UNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The magnitude
More informationBUCKLING AND POSTBUCKLING ANALYSIS OF SHELLS UNDER QUASISTATIC AND DYNAMIC LOADS
BUCKLING AND POSTBUCKLING ANALYSIS OF SHELLS UNDER QUASISTATIC AND DYNAMIC LOADS R. Degenhardt, H. Klein, A. Kling, H. Temmen, R. Zimmermann DLR Institute of Structural Mechanics Lilienthalplatz 7, 388
More informationBuckling Resistance Assessment of a Slender Cylindrical Shell Axially Compressed
Mechanics and Mechanical Engineering Vol. 14, No. 2 (2010) 309 316 c Technical University of Lodz Buckling Resistance Assessment of a Slender Cylindrical Shell Axially Compressed Jakub Marcinowski Institute
More informationMECHANICS OF MATERIALS
00 The McGrawHill Companies, Inc. All rights reserved. T Edition CHAPTER MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Teas Tech Universit
More informationFLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION N. V. De Carvalho 1*, B. Y. Chen
More informationShafts: Torsion of Circular Shafts Reading: Crandall, Dahl and Lardner 6.2, 6.3
M9 Shafts: Torsion of Circular Shafts Reading: Crandall, Dahl and Lardner 6., 6.3 A shaft is a structural member which is long and slender and subject to a torque (moment) acting about its long axis. We
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationNUMERICAL SIMULATIONS OF CORNERS IN RC FRAMES USING STRUTANDTIE METHOD AND CDP MODEL
Numerical simulations of corners in RC frames using StrutandTie Method and CDP model XIII International Conference on Computational Plasticity. Fundamentals and Applications COMPLAS XIII E. Oñate, D.R.J.
More informationInitial Stress Calculations
Initial Stress Calculations The following are the initial hand stress calculations conducted during the early stages of the design process. Therefore, some of the material properties as well as dimensions
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationMECHANICS OF MATERIALS. Prepared by Engr. John Paul Timola
MECHANICS OF MATERIALS Prepared by Engr. John Paul Timola Mechanics of materials branch of mechanics that studies the internal effects of stress and strain in a solid body. stress is associated with the
More informationThe design of a formula student front impact attenuator
The design of a formula student front impact attenuator J.M.J. Schormans MT 10.06 Supervisors: dr. ir. Varvara Kouznetsova Eindhoven University of Technology Department of Mechanical Engineering Computational
More informationStress Analysis of Radial and Non Radial Nozzle Connections in Ellipsoidal Head Pressure Vessel
Journal of Mechanical Engineering Vol. 10, No. 1, 6783, 2013 Stress Analysis of Radial and Non Radial Nozzle Connections in Ellipsoidal Head Pressure Vessel Haszeme Abu Kasim 1, a Professor Dr. Ir. Wahyu
More informationAN ALTERNATIVE TECHNIQUE FOR TANGENTIAL STRESS CALCULATION IN DISCONTINUOUS BOUNDARY ELEMENTS
th PanAmerican Congress of Applied Mechanics January 0408, 00, Foz do Iguaçu, PR, Brazil AN ALTERNATIVE TECHNIQUE FOR TANGENTIAL STRESS CALCULATION IN DISCONTINUOUS BOUNDARY ELEMENTS Otávio Augusto Alves
More informationExperimental Study and Numerical Simulation on Steel Plate Girders With Deep Section
6 th International Conference on Advances in Experimental Structural Engineering 11 th International Workshop on Advanced Smart Materials and Smart Structures Technology August 12, 2015, University of
More informationCHAPTER 6: ULTIMATE LIMIT STATE
CHAPTER 6: ULTIMATE LIMIT STATE 6.1 GENERAL It shall be in accordance with JSCE Standard Specification (Design), 6.1. The collapse mechanism in statically indeterminate structures shall not be considered.
More informationOPTIMAL DESIGN OF COMPOSITE INSERTS FOR A HYBRID ULTRACENTRIFUGE ROTOR
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS OPTIMAL DESIGN OF COMPOSITE INSERTS Hak Gu Lee 1*, Jisang Park 1, Ji Hoon Kim 1 1 Composite Materials Group, KIMS, Changwon, Korea * Corresponding
More informationMarch 24, Chapter 4. Deflection and Stiffness. Dr. Mohammad Suliman Abuhaiba, PE
Chapter 4 Deflection and Stiffness 1 2 Chapter Outline Spring Rates Tension, Compression, and Torsion Deflection Due to Bending Beam Deflection Methods Beam Deflections by Superposition Strain Energy Castigliano
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationA PAPER ON DESIGN AND ANALYSIS OF PRESSURE VESSEL
A PAPER ON DESIGN AND ANALYSIS OF PRESSURE VESSEL P.Palanivelu 1, R.Siva Prasad 2, 1 PG Scholar, Department of Mechanical Engineering, Gojan School of Business and Technology, Redhills, Chennai, India.
More informationGerald Allen Cohen, 83, passed away Oct. 1, 2014, at his home in Laguna Beach.
Dr Gerald Allen Cohen (19312014) Ringstiffened shallow conical shell designed with the use of FASOR for NASA s Viking project in the 1970s. (from NASA TN D7853, 1975, by Walter L. Heard, Jr., Melvin
More informationTorsion of Solid Sections. Introduction
Introduction Torque is a common load in aircraft structures In torsion of circular sections, shear strain is a linear function of radial distance Plane sections are assumed to rotate as rigid bodies These
More informationFailure Mode Predictions in the Compressive Response of Laminated Composites
Structures, Structural Dynamics, and Materials and Colocated Conferences April 811, 2013, Boston, Massachusetts 54th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference AIAA
More informationBuckling Stability of Thin Walled Cylindrical Shells Under Axial Compression
Failure of Engineering Materials & Structures Code 48 UET TAXILA MECHNICAL ENGINEERING DEPARTMENT Buckling Stability of Thin Walled Cylindrical Shells Under Aial Compression Himayat Ullah 1 and Sagheer
More informationNumerical Stability Analysis of Composite Plates Thermally Stiffened by Finite Element Method
Proceedings of COBE 005 Copyright 005 by ABC 8th International Congress of echanical Engineering ovember 6, 005, Ouro Preto, G umerical Stability Analysis of Composite Plates hermally Stiffened by Finite
More informationA FINITE ELEMENT MODEL FOR THE ANALYSIS OF DELAMINATIONS IN FRP SHELLS
TRENDS IN COMPUTATIONAL STRUCTURAL MECHANICS W.A. Wall, K.U. Bletzinger and K. Schweizerhof (Eds.) c CIMNE, Barcelona, Spain 2001 A FINITE ELEMENT MODEL FOR THE ANALYSIS OF DELAMINATIONS IN FRP SHELLS
More informationParametric Instability and SnapThrough of Partially Fluid Filled Cylindrical Shells
Available online at www.sciencedirect.com Procedia Engineering 14 (011) 598 605 The Twelfth East AsiaPacific Conference on Structural Engineering and Construction Parametric Instability and SnapThrough
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More informationINTRODUCTION TO THE EXPLICIT FINITE ELEMENT METHOD FOR NONLINEAR TRANSIENT DYNAMICS
INTRODUCTION TO THE EXPLICIT FINITE ELEMENT METHOD FOR NONLINEAR TRANSIENT DYNAMICS SHEN R. WU and LEI GU WILEY A JOHN WILEY & SONS, INC., PUBLICATION ! PREFACE xv PARTI FUNDAMENTALS 1 1 INTRODUCTION 3
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More information